Development, Characterization and Applications of a Non
Proprietary Ultra High Performance Concrete for
Sherif El-Tawil, Mouhamed Alkaysi, Antoine E. Naaman, Will Hansen
and Zhichao Liu
Department of Civil and Environmental Engineering
University of Michigan, Ann Arbor, Michigan
Intentionally left blank
1. Report No.
2. Government Accession No.
3. MDOT Project Manager Steve Kahl
4. Title and Subtitle
Development, Characterization and Applications of a Non Proprietary Ultra High Performance Concrete for Highway Bridges
5. Report Date 03/14/2016
6. Performing Organization Code N/A
Sherif El-Tawil, Mouhamed Alkaysi, Antoine E. Naaman, Will Hansen and Zhichao Liu
8. Performing Org. Report No.
N/A 9. Performing Organization Name and Address
University of Michigan
Room 1038 Wolverine Tower 3003 South State Street Ann Arbor, MI 48109
10. Work Unit No. (TRAIS) N/A
11. Contract No.
11(a). Authorization No.
Z1 12. Sponsoring Agency Name and Address
Michigan Department of Transportation Research Administration
8885 Ricks Rd.
P.O. Box 30049 Lansing MI 48909
13. Type of Report & Period Covered
3/30/2013 – 3/14/2016 14. Sponsoring Agency Code N/A
15. Supplementary Notes N/A
Ultra-high performance concrete (UHPC) is a new class of cementitious materials that have exceptional mechanical and durability characteristics. UHPC is commercially available.
However, its cost for construction of highway structures is prohibitive. Based on an extensive testing program, a new family of non-proprietary UHPC materials with excellent characteristics in compression and tension, as well as exceptional resistance to freeze-thaw and chloride ion penetration were developed. The most cost effective of these deviates from traditional UHPC mixtures in that it uses a 50:50 mix of Portland Type I and Ground Granulated Blast-Furnace Slag (GGBS) as a binder, lacks any silica powder (inert filler) and requires no post-placement treatment. The use of GGBS improves the material’s ‘greenness’ making it a more sustainable cementitious product. Specifications for making the new UHPC were proposed. The developed UHPC blend was then used to conduct a comprehensive study on bond between UHPC and deformed steel bars to facilitate and enable future structural applications. Bond pull out tests showed the developed UHPC requires significantly reduced development lengths in order to attain steel bar yield compared to traditional concrete. Models to characterize the bond strength were proposed and a UHPC joint consisting of two pre-cast bridge deck elements was developed and tested at full scale. It was shown that a 6” (150 mm) joint made of the developed UHPC was sufficient to successfully transfer loading between the decks.
17. Key Words
Ultra-high performance concrete, non-proprietary, durability, strength, bond, joints, precast concrete, bridge, freeze-thaw
18. Distribution Statement
No restrictions. This document is available to the public through the Michigan Department of Transportation.
19. Security Classification - report
20. Security Classification - page Unclassified
21. No. of Pages 22. Price N/A
Intentionally left blank
This publication is disseminated in the interest of information exchange. The Michigan Department of Transportation (hereinafter referred to as MDOT) expressly disclaims any liability, of any kind, or for any reason, that might otherwise arise out of any use of this publication or the information or data provided in the publication. MDOT further disclaims any responsibility for typographical errors or accuracy of the information provided or contained within this information. MDOT makes no warranties or representations whatsoever regarding the quality, content, completeness, suitability, adequacy, sequence, accuracy or timeliness of the information and data provided, or that the contents represent standards, specifications, or regulations.
Intentionally left blank
This project was funded by the Michigan Department of Transportation. The authors would like to acknowledge the support and efforts of Mr. Steve Kahl and Mr. David Juntunen for initiating and directing this research. The authors also wish to acknowledge the continuing assistance of the Research Advisory Panel (RAP) members in contributing to the advancement of this study.
The authors acknowledge the help and ideas of Prof. Kay Wille of the University of Connecticut, Storrs, who served as a consultant on this project. Parts of this work were conducted by the second author in fulfillment of his PhD dissertation requirements at the University of Michigan.
Intentionally left blank
Table of Contents
List of Figures ... 5
List of Tables ... 9
EXECUTIVE SUMMARY ... 1
1. INTRODUCTION ... 5
1.1. Ultra-High Performance Concrete (UHPC) ... 5
1.2. Research Objectives ... 5
1.3. Organization of the Report ... 7
2. BACKGROUND AND LITERATURE REVIEW ... 9
2.1. Strength of UHPCs ... 9
2.1.1. Compressive and Tensile Behavior of UHPC ... 9
2.1.2. Effect of Silica Fume ... 10
2.1.3. Effect of Silica Powder ... 11
2.1.4. Cements Effects on UHPCs ... 11
2.1.5. Effect of Fiber Type and Quantity ... 12
2.2. DURABILITY OF UHPCs ... 12
2.2.1. Freeze-Thaw Resistance ... 12
2.2.2. Chloride Ion Penetration Resistance: ... 13
2.3. Bond Development in UHPCs ... 14
2.3.1. Bond Development of Steel Bars Embedded in UHPC ... 14
2.3.2. Lap Splice & Component Tests with UHPC ... 15
3. MATERIAL PERFORMANCE AND CHARACTERIZATION ... 17
3.1. OVERVIEW ... 17
3.2. EXPERIMENTAL PARAMETERS AND PROCEDURE ... 18
3.2.1. UHPC Material Properties and Cost ... 18
3.2.2. Steel Fibers ... 21
3.2.3. Mixing Procedure ... 22
3.2.4. Tensile Strength Testing: ... 23
3.2.5. Compression Testing: ... 25
3.3. RESULTS AND DISCUSSION ... 26
3.3.1. Analysis of Data ... 26
3.3.2. Overview of Results ... 27
3.3.3. Cement Type ... 29
3.3.4 - Silica Powder ... 30
3.3.4. Silica Fume ... 33
3.3.5. Fiber Content ... 35
3.3.6. Cost Analysis ... 39
3.4. CONCLUSION ... 40
4. DURABILITY PERFORMANCE OF UHPC ... 43
4.1. OVERVIEW ... 43
4.2. EXPERIMENTAL PARAMETERS ... 43
4.2.1. UHPC Mix Designs ... 43
4.2.2. Experimental Procedure ... 45
4.2.3. Air Void Analysis ... 47
4.2.4. Rapid Chloride Penetration Test ... 48
4.2.5. Compressive Strength Testing ... 49
4.3. EXPERIMENTAL RESULTS ... 49
4.3.1. Freeze-Thaw Resistance ... 49
4.3.2. Air Void Analysis ... 53
4.3.3. Rapid Chloride Permeability ... 56
4.4. DISCUSSION OF EXPERIMENTAL RESULTS ... 59
4.5. CONCLUSION ... 62
5. FACTORS AFFECTING BAR BOND DEVELOPMENT FOR UHPC ... 65
5.1. OVERVIEW ... 65
5.2. EXPERIMENTAL PARAMETERS AND PROCEDURE: ... 65
5.2.1. Bar Pull Out Testing Program and Test Set Up ... 65
5.2.2. Lap Splice Joint Testing Program ... 69
5.2.3. Material Properties ... 71
5.2.4. Bar Pull Out Results ... 72
5.2.5. Effect of Embedment Length ... 74
5.2.6. Effect UHPC Cast Orientation on Bond ... 81
5.2.7. Effects of Fiber Volume Content ... 83
5.2.8. Early Age Testing of UHPC on Bond ... 84
5.2.9. Bar Pull Out vs. Lap Splice Beam Results ... 86
5.2.10. Design Implications ... 88
5.3. CONCLUSION ... 89
6. SIMPLIFIED UHPC JOINTS FOR BRIDGE CONSTRUCTION ... 93
6.1. OVERVIEW ... 93
6.2. DESIGN OF THE EXPERIMENTAL PROGRAM ... 93
6.2.1. Pure Flexure vs. Combined Shear and Flexure Testing ... 94
6.2.2. Joint Details & Selection ... 95
6.2.3. Specimen Design ... 96
6.2.4. Specimens Tested and Material Parameters ... 98
6.3. EXPERIMENTAL PROCEDURE ... 100
6.3.1. Test Set Up ... 100
6.3.2. Instrumentation ... 100
6.4. MATERIALS ... 101
6.5. CONSTRUCTION OF THE PRECAST CONCRETE SPECIMENS ... 102
6.6. RESULTS AND DISCUSSION ... 104
6.6.1. Comparison of Calculated Bar Stress versus Measured Bar Stress ... 104
6.6.2. F-100 Specimen Tests ... 105
6.6.3. F-150 and F-200 Specimens ... 106
6.6.4. Effect of Fiber Content in Pure Flexure ... 108
6.6.5. Effect of Joint Size ... 109
6.6.6. Combined Shear and Flexure Testing ... 110
6.6.7. Effect of Fiber Content in Combined Shear and Flexure ... 111
6.7. FINITE ELEMENT MODEL AND PARAMETRIC STUDY ... 112
6.7.1. Model Setup ... 112
6.7.2. UHPC and Concrete Material Models ... 113
6.7.3. Parametric Study ... 115
6.7.4. Model Validation ... 116
6.7.5. Results of Parametric Study ... 116
6.8. CONCLUSION ... 119
7. SUMMARY, MAJOR CONCLUSIONS AND FUTURE RESEARCH ... 121
7.1. SUMMARY AND MAJOR CONCLUSIONS ... 121
7.2. PROMISE AND COMMERCIAL POTENTIAL OF UHPC ... 122
7.3. AN OPPORTUNITY FOR THE STATE OF MICHIGAN ... 123
7.4. A BRIGHT FUTURE ... 123
7.5. FUTURE RESEARCH NEEDS ... 124
8. REFERENCES ... 125
9. APPENDIX A – STRESS-STRAIN PLOTS FOR ALL UHPC MIXES ... 135
9.1. WHITE CEMENT MIXES ... 136
9.2. PORTLAND TYPE V CEMENT MIXES ... 139
9.3. GGBS/PORTLAND TYPE I CEMENT MIXES ... 142
10. APPENDIX B – RESULTS OF FREEZE-THAW TESTING – RILEM ... 143
11. APPENDIX C – DETAILS FROM BAR PULL-OUT TESTING ... 145
12. APPENDIX D – DETAILS OF BEAM TESTING ... 177
13. APPENDIX E – SPECIAL PROVISIONS ... 195
v List of Figures
Figure 2-1 Typical Tensile Strain Response in UHPC ... 10
Figure 3-1 Grain Size Analysis for Sand ... 19
Figure 3-2: Example of the Steel Fibers Used in this Study ... 22
Figure 3-3 Mixing process (photos courtesy of Prof. Kay Wille) ... 23
Figure 3-4 Tensile test set up, (b) Instrumentation, (c) Specimen dimensions ... 24
Figure 3-5: Tensile and Compression Specimens Post Test ... 26
Figure 3-6: Effects of Different Cements on UHPC for Mixes with 1.5% Volume Fiber Content ... 31
Figure 3-7: Effects of Silica Powder Contents on UHPC for Mixes with 1.5% Volume Fiber Content ... 32
Figure 3-8: Effect of Silica Fume Contents on UHPC for Mixes with 1.5% Volume Fiber Content ... 34
Figure 3-9: Effects of Lower Steel Fiber Volume Contents on UHPC ... 36
Figure 3-10: Strain Response for UHPC Specimens in Tension ... 38
Figure 3-11: Strain (%) Capacity as function of Steel Fiber Content ... 39
Figure 3-12: Compressive Strength as a function of Cost Index ... 40
Figure 4-1: Freeze Thaw Test Close-Up (17) ... 46
Figure 4-2: Specimen with Test Surface Facing the Bottom under Frozen Condition ... 46
Figure 4-3: Temperature Profile of Freeze-Thaw Test ... 47
Figure 4-4: Treated and Untreated UHPC Cross Section for Air Void Analysis ... 48
Figure 4-5: Mass Loss of UHPC Mixes after at Least 60 Cycles ... 51
Figure 4-6: a. Effect of Silica Powder on Mass Loss; b. Average Mass Loss as a Function of Silica Powder Quantity ... 52
Figure 4-7: Average Mass Loss as a Function of Cement Type ... 52
Figure 4-8: Air Content by LTM and PCM ... 54
Figure 4-9: Air Content as a Function of Power’s Spacing Factor ... 55
Figure 4-10: a. Air Content as a Function of Silica Powder Percent, b. Average Air Content as a function of Silica Powder ... 56
Figure 4-11: Average Air Content as a Function of Cement Type ... 56
Figure 4-12: Total Charge Passed for UHP C and RC Mix ... 57
Figure 4-13: a. Total Coulombs passed as a function of Silica Powder Percent; b. Average Coulombs passed as a function of Silica Powder ... 58
Figure 4-14: Average Coulombs passed as a function of Cement Type ... 59
Figure 4-15: Particle Size Distributions for UHPC Mixes and Regular Concrete ... 61 Figure 4-16: Moisture Uptake and RDM% for UHPCs (27) ... 62 Figure 5-1: (a) Test Set Up for Bar Pull Out (b) and Instrumentation and Load Path for Specimen ... 66 Figure 5-2: (a) Fibers Aligned Parallel to Bar (b) Fibers Aligned Transversely to Bar ... 68 Figure 5-3: Construction and Reinforcement Details for Precast Decks with UHPC Joint ... 70 Figure 5-4: Four Point Bending Test Set Up for Flexure Test for Specimens F-100-1P-1, F-100- 1P-2, F-100-2P-1 and F-100-2P-2 ... 71 Figure 5-5: (a) Bar Fracture, (b) Bar Slip, and (c) Conical Concrete Failure ... 72 Figure 5-6: Force Slip for 13 mm bars at (a) 100 mm, (b) 75 mm, and (c) 50 mm embedment, (d) Peak Bond Stress vs. Embedment Length ... 76 Figure 5-7: Idealized Reaction of Reinforcing Steel Embedded in Concrete, Subjected to Tension, Cross Sectional View ... 77 Figure 5-8: Force Slip for 16 mm bars at (a) 100 mm, (b) 75 mm, and (c) 50 mm embedment, (d) Peak Bond Stress vs. Embedment Length ... 78 Figure 5-9: Force Slip for 19 mm bars at (a) 100 mm, (b) 75 mm, and (c) 50 mm embedment, (d) Peak Bond Stress vs. Embedment Length ... 80 Figure 5-10: (a) Comparison of Bond Data for 16 mm Epoxy Coated Bar and (b) scatter of the current data available for 13 mm, 16 mm, and 19 mm bars ... 82 Figure 5-11: (a) Force Slip for 16mm bars with Parallel and Transverse Fibers, (b) Force Slip for 19 mm bars with Parallel and Transverse Fibers, and (c) Bond Stress Comparison (Dark Gray- 19 mm bars, Light Gray – 16 mm bars) ... 83 Figure 5-12: (a) Force Slip for 16 mm bars with 1% and 2% Fibers, (b) Force Slip for 19 mm bars with 1% and 2% Fibers, and (c) Bond Stress Comparison (Dark Gray – 19 mm bars, Light Gray – 16 mm bars) ... 85 Figure 5-13: (a) Force-Slip Curve, (b) Bond Stress – Relative Slip, (c) Compressive Strength and (d) Bond Stress Data for Early Age Tests ... 86 Figure 5-14: Average Bond Stresses in lap splices vs. bar pull out specimens. ... 88 Figure 5-15: Maximum Average Bar Stress under Direct Pull Out ... 89 Figure 6-1: Shear and Moment forces in beams under (a) pure flexure loading and (b) combined shear and flexure testing ... 95 Figure 6-2: Joint Dimensions and Reinforcement Details ... 97 Figure 6-3 Joint Shape Details for the 150 mm (a), 200 mm (b) joint, Lap Splice Connection Detail (c) ... 99 Figure 6-4: Instrumentation of the Precast Bridge Deck Beams ... 101 Figure 6-5: Deformed 16 mm Epoxy Reinforcement Bar ... 102
Figure 6-6: Forms and Placed Bars (a), Lap Splice (b), Poured UHPC Joint (c), and Set up with DIC (d) ... 103 Figure 6-7: Comparison of Calculated and Measured Bar Stresses ... 105 Figure 6-8: (a) DIC of 100 mm joint specimens, (b) Splitting Failure in deformed specimen, (c) Load-Deflection Curves for 100 mm specimens with 2% fibers and (d) 100 mm specimens with 1% fibers. ... 106 Figure 6-9: (a) DIC of 150 mm joint specimens, (b) Splitting Failure in deformed specimen, (c) Load-Deflection Curves for 150 mm specimens and (d) 200 mm specimens. ... 108 Figure 6-10: Maximum Force in F-100 Decks at a Function of Fiber Volume Content ... 109 Figure 6-11: Moment at Joint as a function of Joint Width ... 110 Figure 6-12: (a) DIC of 100 mm joint, SF specimens, (b) Splitting Failure in deformed specimen, (c) Load-Deflection Curves for 100 mm specimens, 1% fiber by vol. and (d) 100 mm specimens, 2% fiber by vol. ... 112 Figure 6-13: (a) Finite Element Model and (b) Mesh for F-150-2P Specimens ... 113 Figure 6-14: Typical UHPC Tensile Response for Joint Fill Material ... 114 Figure 6-15: (a) Original Joint Design for FEA, (b) non-tapered joint design, and (c) flat joint design. ... 115 Figure 6-16: Experimental FEA Load-Deflection for (a) 150 mm joints and (b) 200 mm joints ... 118 Figure 6-17: (a) Un-deformed shape, (b) deformed shape and (c) von Mises Strain for 150 mm, (d) Plot of the cracks developed and (e) and Damaged Beam after Testing, Actual joint ... 118
Intentionally left blank
ix List of Tables
Table 3-1: Chemical and Physical Properties of Materials ... 19
Table 3-2: Mixture Proportions by Weight with Cost Index ... 20
Table 3-3: Cement Properties ... 21
Table 3-4: Cost and Performance Summary ... 28
Table 3-5: UHPC Mix Design and Ratios ... 40
Table 4-1: Mixes Proportions for UHPCs tested ... 44
Table 4-2: Summary of Test Results ... 50
Table 4-3: Chloride Permeability Rating ... 57
Table 5-1: Experimental Parameters and Number of Tests ... 69
Table 5-2: Test Results for Simple Bar Pull Out ... 73
Table 5-3: Test Results Beam Lap Splice Tests ... 87
Table 6-1: Main Variable of Beam Specimens ... 99
Table 6-2: Summary of Results from Experimental Testing ... 104
Table 6-3: Material Parameters for FEM ... 114
Table 6-4: Summary of Simulated Beams ... 116
Intentionally left blank
1 EXECUTIVE SUMMARY
Ultra-high performance concrete (UHPC) is a cementitious material that achieves a compressive strength of at least 22 ksi (150 MPa) and has self-consolidation properties. It is comprised of component materials with particle sizes and distributions carefully selected to maximize packing density. The high packing density, which means that constituent particles are arranged as compactly as possible, is the reason for the extremely high mechanical and durability properties of the material.
UHPC is commercially available at the present time. However, its cost for construction of highway structures is prohibitive. A non-proprietary version of UHPC was recently developed at the University of Michigan (UM). While significantly cheaper than the cost of commercial products, the cost of the UM version is still relatively high and can be substantially reduced through optimization of its constituent components while still maintaining the extraordinary properties that make UHPC such an exceptional building material.
The primary objective of this project is to develop a cost-optimized version of non-proprietary UHPC and characterize its mechanical and durability properties. Another key objective is to investigate the possibility of using UHPC for field-cast joints that commonly occur in precast construction. Specific objectives include:
• Identify a low cost, non-proprietary UHPC mix design through cost-optimization of the constituent components while still maintaining the exceptional properties of UHPC.
• Characterize the strength and durability properties of the optimized mixture, focusing specifically on tensile and compressive strengths, freeze-thaw resistance and rapid chloride penetration resistance.
• Quantify the bond between UHPC and deformed steel bar reinforcement for a range of parameters and loading scenarios associated with feasible bridge applications.
• Investigate the use of UHPC bridge field joints between precast regular concrete decks.
Summary of Research:
Some of the component materials of UHPC are substantially more expensive than those used in regular concrete. To optimize cost, research was conducted to investigate the relationship between material performance and the type or amount of the most expensive components, i.e.
cement, silica fume and silica powder. Short-term material performance was assessed via tensile and compressive tests and durability properties were evaluated based on freeze-thaw and chloride ion penetration testing as well as quantification of the presence and distribution of air voids. The test results were used to optimize cost versus performance characteristics of the UHPC blends considered. At the structural level, a comprehensive study investigating the bonding between UHPC and deformed bars was carried to investigate the effect on bond of bar size, type, embedded length, fiber content, fiber orientation and curing age. Using this data, new joints making use of UHPCs superior bond characteristics were constructed and tested in order to prove a quick and simple method for the assembly of precast bridge elements.
Summary of Results:
From the material testing program, a low cost UHPC material with excellent characteristics in compression and tension, as well as exceptional resistance to freeze-thaw and chloride ion
penetration was developed. The proposed mix deviates from traditional UHPC mixtures in that it uses a 50:50 mix of Portland Type I and Ground Granulated Blast Furnace Slag (GGBS) as a binder, lacks any Silica Powder (inert filler) and requires no post-placing treatment. The cost of the cementitious material ingredients was reduced by half compared to available non-proprietary UHPCs available at the onset of this research. The use of GGBS improves the material’s
‘greenness’ making it a more sustainable cementitious product. Specifications for making the new UHPC were proposed.
The developed UHPC blend was then used to conduct a comprehensive study on bond between UHPC and deformed steel bars to facilitate and enable future structural applications. Bond pull out tests showed the developed UHPC requires significantly reduced development lengths in order to attain steel bar yield compared to traditional concrete. Models to characterize the bond strength were proposed and a UHPC joint consisting of two pre-cast bridge deck elements was developed and tested. It was shown that a 150 mm (6 inch) joint was sufficient to successfully transfer loading between the decks.
The Promise of UHPC - An Opportunity for the State of Michigan:
UHPC derives its unique properties from its high packing density and the presence of steel fibers. The special constituents of UHPC make it more expensive than regular concrete.
However, they also give it its exceptional short- and long-term properties. In particular, the extremely high freeze-thaw resistance, negligible chloride penetration, and ability to mobilize the material’s strain hardening response in tension to limit crack width, suggests that UHPC structures can be extremely long-living and low maintenance at the same time. Such structures will have inherently low life cycle costs, in spite of relatively higher initial costs.
UHPC is currently in its infancy and this project is an important early step. Additional research on fiber optimization, mixing technology and structural testing is needed to fully realize the material’s promise. These research topics represent an opportunity for the State of Michigan to take leadership in steel fiber production, a key component of UHPC. The State, with its focus on vehicle manufacturing, is well suited to be major fiber industry hub given that steel fibers are made from chopped high strength wires that are used in steel-belted tire products.
5 1. INTRODUCTION
1.1. Ultra-High Performance Concrete (UHPC)
Ultra-high performance concrete is a new class of cementitious materials that achieve a compressive strength of at least 22 ksi (150 MPa) (Wille et al. 2014, Graybeal 2014, Wille et al.
2012, Wille et al. 2011). When properly reinforced with steel fibers, UHPCs can achieve strain hardening behavior and display compressive and direct tensile strengths as high as 35 ksi (242 MPa) and 2 ksi (14 MPa), respectively (Graybeal, 2003). Changes in the type and quantity of steel fibers directly affect the ductility, durability and strength of the material (Wille et al. 2011;
Kim et al. 2011, 2010a, 2010b, 2010c, 2008a, 2008b, 2008c, 2008d, 2007). UHPC also exhibits exceptional energy absorption prior to crack localization (Pyo et al. 2015a, 2015b, 2013a, 2013b, 2013c) and self-consolidation properties (Graybeal, 2006).
Recent developments in UHPC at the University of Michigan have led to new, non-proprietary formulations that are cheaper than the patented versions (Wille et al, 2011). The new formulation described in Wille et al. (2011) is made up of components readily available on the US open market, does not require any special mixing or placing equipment and has a higher ductility than other commercially available products (Rigaud et al., 2012). Relative to traditional concretes, the price of the non-proprietary UHPC in Wille et al. (2011) remains high, but still it is substantially less than its patented commercial equivalent.
1.2. Research Objectives
With strengths in compression approaching that of mild steel, finding new uses for UHPCs is intriguing many practitioners, who want to use the material in their projects. However, broad
usage is hindered by the high cost of the material and lack of test results, and understanding in general, of UHPCs behavior at the structural level. With these issues in mind, the objectives of this research project are:
• Survey and identify potential applications for non-proprietary UHPC particularly for Accelerated Bridge Construction (ABC) and Precast Bridge Element Systems (PBES).
• Investigate whether a family of new UHPC materials can be made using locally available components and optimize the cost by tailoring of the mix, while still maintaining ultrahigh performance characteristics.
• Characterize the properties of the new family of UHPCs, focusing on tensile strength, compressive strength, modulus of elasticity, and durability by laboratory testing.
• Conduct pullout tests of steel reinforcing bars from UHPC to investigate the bond strength between steel bars with various coatings and the surrounding UHPC matrix.
• Investigate using computational and experimental methods to simulate the behavior of UHPC field joints (closure pours).
• Develop detailed guidance (special provisions) for making the proposed UPHC on a construction site.
• Assess the life cycle performance of UHPC in light of the experimental results.
• Propose future research efforts using the developed UHPC.
7 1.3. Organization of the Report
The main body of the report is preceded by detailed contents including lists of figures and tables.
This is followed by an introduction giving briefly the scope and objectives of the study and importance of the topic.
• Chapter 2 outlines the previous works involving UHPC that are of interest to the topics covered in this report.
• Chapter 3 covers an investigation into how material properties change as a result of variations in the amount and/or type of individual components. The chapter aims to optimize the cost of UHPC with respect to its strength.
• Chapter 4 investigates the durability of select UHPC mixes identified in chapter 3 through freeze-thaw testing, rapid chloride penetration testing and air void characterization.
• Chapter 5 gives an in depth study into the factors affecting bond between UHPC and reinforcing steel.
• Chapter 6 studies the use of UHPC in precast bridge constructions via experimental testing and finite element analysis.
• Chapter 7 provides a summary of the research, the most important conclusions and future work.
All chapters are preceded by a brief synopsis of the chapter. References which have been used for certain inputs are listed at the very end of the report.
Intentionally left blank
2. BACKGROUND AND LITERATURE REVIEW
2.1. Strength of UHPCs
2.1.1. Compressive and Tensile Behavior of UHPC
The high compressive strength of UHPC is well known and established (Graybeal, 2014).
Larrard and Sedran (1994) produced a concrete mortar with a compressive strength of 35 ksi (236 MPa). Wille, Naaman and El-Tawil (2011) were able to prepare UHPCs with 28-day compressive strengths in excess of 30 ksi (200 MPa) without requiring the use of expensive post treatment techniques. Graybeal (2006) has shown that UHPC reaches a peak stress of around 22 ksi at 0.003 strains (0.3%). Wille and Namaan (2011) showed that when reinforced with steel fibers, UHPC mixes were able to achieve 0.6% strain capacity in tension prior to strain softening.
More information regarding the tensile and compressive behavior of UHPCs can be found in the works by Wille (2011) and Graybeal (2003, 2006, and 2014).
UHPC not only has a higher tensile strength than conventional concrete, it can also exhibit strain hardening response after initial cracking when properly reinforced with steel fibers. The typical stress strain curve for ultra-high performance concrete is shown in Figure 2-1. Following the definitions set forth by Naaman (Naaman & Reinhardt, 2007), the first part of the material’s tensile behavior is elastic, which continues up until the specimen develops an initial crack at what is known as the first cracking strength point (σcc, εcc) in Figure 2-1. Following this, the material then exhibits strain hardening up until its peak point (σpc, εpc). The strain hardening behavior of segment II is typically characterized by multiple crack development in the gauge length of the specimen. Following the strain-hardening region, the material then begins to exhibit crack localization (segment III). This segment of the curve is best represented by a stress versus
crack opening response but many researchers continue to describe the region as a stress versus strain relationship, based on the nominal gage length of the specimen, as is done herein.
Figure 2-1 Typical Tensile Strain Response in UHPC 2.1.2. Effect of Silica Fume
Most UHPCs contain silica fume and silica powder. Silica fume is a reactive powder with pozzolonic properties. Silica powder is an inert powder, used primarily to increase the density of the cementitious matrix. Several research studies have investigated the effects of silica fume (SF) on the behavior of UHPCs. Rong, Xiao and Wang (2014) investigated the effects of SF on the hydration and microstructure of UHPCs, concluding that SF dominated the hydration process at lower water-binder ratios. Rong et al. (2015) also partially replaced cement with SF in UHPCs and determined the flexural and compressive strengths were highest when the content of SF was approximately 3% to binder, and decreased at higher contents due to the agglomeration of SF particles. Brouwers et al. (2014) similarly investigated the effect of SF on the UHPC hydration
process and material behavior, concluding that an optimal ratio of 3.74% SF to binder yields the highest mechanical properties of UHPC. Oertel et al. (2013) reported that the nearer the dispersion of silica particle sizes match to those in the primary mixture particle sizes, the further the compressive strengths increase in UHPCs. Wille (2015) studied the effects of various SFs on the compressive behavior in UHPCs, and reported compressive strengths ranging from 20 ksi to 26 ksi. To the authors’ knowledge, no work has been done on the effect of silica fume on the direct tensile properties of UHPCs.
2.1.3. Effect of Silica Powder
To date, little work has been done to investigate the effects of Silica Powder (SP) on the tensile and compressive performance of UHPCs. Wille (2011) researched the effects of SP on UHPCs ranging from 0 SP-binder to 0.5 SP-binder ratios, finding a ratio of 0.3 SP to cement yielded the highest compressive strength. As with silica fume, to the knowledge of the authors, no work has been done evaluating the effect of different silica powder quantities in UHPCs under direct tension.
2.1.4. Effect of Cement
Additionally, little work has been done to investigate the effects of various cements on the material behavior of UHPC. Yu and Brouwers (2015) used fly ash (FA), ground granulated blast- furnace slag (GGBS) and limestone powder (LP) to replace cement in UHPC mixes, determining UHPCs with the GGBS has higher mechanical properties at 28 and 91 days than with other cements they considered. Wille (2015) investigated the compressive strengths for UHPCs substituting several different cements, yielding strengths between 19 ksi (130 MPa) and 32 ksi
(221 MPa). To date, no work quantifies the effects of cement type on the tensile response of UHPCs.
2.1.5. Effect of Fiber Type and Quantity
Several papers currently discuss the effects of fiber content, shape, size and topology on ultra- high performance concretes. The addition of steel fibers into the ultra-high performance concrete matrix leads to enhanced material performance such as a high tensile capacity, ductility, reduced crack spacing, and high energy dissipation capability. The magnitude of these effects is a direct result of the fiber material strength, cementitious matrix – fiber bond ability, fiber aspect ratio (length: diameter), fiber volume content and fiber surface topology. Pyo (2015) investigated the strain rate dependent tensile properties of UHPCs with different fibers and fiber volume contents.
Wille (2011) investigated the tensile performance of UHPCs with fiber contents as low as 1%.
Yu and Brouwers (2015) investigated hybrid fiber UHPCs containing a combination of hooked, short and long straight fibers, at 2% volume contents. They concluded that the combination of several fiber types yields ultra-high performance while using fewer fibers. To date, no work has been done investigating the effect of low fiber contents (<1%) on the compressive and tensile performance of UHPC.
2.2. DURABILITY OF UHPCs 2.2.1. Freeze-Thaw Resistance
Tests investigating UHPCs resistance to freeze-thaw have been limited. Ahlborn et al. performed freeze-thaw cycling tests in accordance to ASTM C 666 (2008), procedure B, showing that after 32 freeze-thaw cycles, ultra-high performance concrete specimens showed no degradation. Acker and Behloul (2004) similarly reported that after 300 freeze-thaw cycles, UHPC showed no
degradation. Pierard et al. (2012) reported that specimens achieving strength between 20.3 ksi (140 MPa) and 23.2 ksi (160 MPa) also showed no degradation after 112 cycles. Graybeal (2006) performed air void analyses on Ductal©, finding UHPC void numbers to be between 0.2 and 7.5 voids/in (0.008 and 0.30 voids/mm), corresponding to an air content of 5.7% to 7.3%
with no vibration.
To date, no research has been done to investigate the durability parameters for a non-proprietary blend of UHPC. Further, no testing has been done to investigate the effects of various material parameters on the durability of UHPC. Yazici (2008) looked into the effect of silica fume and high-volume Class C fly ash on the durability of self-compacting concretes, determining that a 10% by volume inclusion of silica fume resulted in enhanced freeze-thaw resistance, accompanied by increased compressive strengths. Work by Alexander and Magee (1999) evaluated the durability of concretes containing condensed silica fumes and ground granulated blast furnace slag (GGBS), determining blends containing these materials outperformed regular concretes in durability testing of water absorption.
2.2.2. Chloride Ion Penetration Resistance:
Performing rapid chloride permeability tests, Ahlborn (2008) showed that UHPC was capable of achieving permeability values less than 100 coulombs for both air-cured and steam-cured specimens. Materials with coulomb values less than 100 are generally considered to have negligible chloride ion penetration. Testing two different types of reactive powder concretes, Bonneau (1997) showed that specimens were able to achieve 6 to 9 coulombs. Graybeal (2006) reported that untreated specimens achieved coulomb values of 360 and 76 at 28 days and 56 days respectively. Most of the existing chloride permeability studies pertain to proprietary materials and data for non-proprietary blends is lacking at present.
14 2.3. Bond Development in UHPCs
2.3.1. Bond Development of Steel Bars Embedded in UHPC
There is limited published data on the bonding behavior between UHPCs and steel reinforcement bars. Graybeal (2010, 2014) performed pull out tests for #4, #5, and #6 bars embedded 3, 4 and 5 inches (75, 100 and 125 mm) respectively into UHPC cylinders, with all of the steel bars fracturing before bond failure. Graybeal (2014) recently has shown that under static conditions, UHPC specimens are capable of developing a bond stresses of approximately 2.9 - 5 ksi (20 – 35 MPa) in bar pull out specimens and are largely dependent on bar spacing, concrete cover, and development length and bar size. In a different study, Swenty and Graybeal (2012) performed pull out tests on #4 bars embedded into 6 in (150 mm) concrete cubes. Two different UHPC mixes were used, one achieving bar fracture and the other achieving bar yield. Performing pull out tests on 12 mm diameter bars, varying concrete cover and embedment lengths, Fehling et al.
(2012) determined that increasing cover widths and embedment lengths increased the bond stress, reaching those sufficient for bar yield. Holschemacher et al. (2004) reported achieving bond stresses up to 8.7 ksi (60 MPa) using 12 mm bars in UHPC cylinders. Saleem et al. (2013) investigated the development length requirements for high strength steel bars in UHPC, concluding that 10 mm and 22 mm (#3 and #7 U.S. sizes) bars require 12 db and 18 db to develop adequately. Jungworth et al. (2004) performed tests on 20 mm and 12 mm diameter bars, reaching bond stresses of 5.5 ksi (38 MPa) and 9.5 ksi (66 MPa). Of the literature currently available on bond, data only exists on testing performed using Ductal® or Ceracem®, both proprietary concretes No published data currently exists for non-proprietary UHPCs. As discussed later on, there is much discrepancy in existing data regarding the maximum achieved
bond stress during the pull out tests, with some studies reporting values as high as 9.5 ksi (66 MPa), or as a low as 1.4 ksi (9.8 MPa) (Graybeal, 2010).
2.3.2. Lap Splice & Component Tests with UHPC
Component level testing with UHPC remains largely confined to highway infrastructure projects.
The Federal Highway Administration has released several reports on test installations on existing structures. UHPC was used in concrete waffle slab decks in an accelerated bridge construction in Wapello County, Iowa showing that UHPC is a viable material for infrastructure redesign (Wipf et al, 2011). New York D.O.T. also tested a live installation of a UHPC joint using hooked bars and a small joint width, also concluding exceptional joint performance for the UHPC (FHWA, 2014).
Steinberg et. al. (2010) investigated the structural reliability of pre-stressed UHPC flexure models for bridge girders showing that acceptable levels of reliability can be obtained using typical AASHTO procedures. Graybeal (2014) released a series of tests evaluating the joint force transfer capacity of UHPC under various parameters, including type of bars, size of bars etc. He concluded that UHPC was able to act as a closure pour joint between two precast decks more efficiently than traditional grouts and concretes at splice lengths as little as 6 inches (150 mm).
Of these tests performed so far, all of them have made use of Ductal.
Few studies have investigated the splice length requirements for UHPC joints. Graybeal recently investigated the splice length of pre-stressing strands in field cast UHPC connections, concluding that 12 mm and 15 mm diameter strands require 20 inches (510 mm) and 24 inches (610 mm) to fully develop (Graybeal, 2015). Hoonhee and Park (2014) investigated the lower limits of contact splice lengths in precast, steam-cured UHPC beams under flexure, determining a lap
splice length greater than 6 in. (150 mm) was required to cause yield in the bars. Both of these studies were performed using Ductal, i.e. no studies currently exist for non-proprietary UHPCs, as provided herein. Furthermore, to the author’s knowledge no studies exist investigating the UHPC’s performance in non-contact lap splices between two precast beam elements, as done herein.
3. MATERIAL PERFORMANCE AND CHARACTERIZATION
This chapter investigates the performance of several new UHPC mix designs with a focus on minimizing cost. Performance parameters include compressive strength and full tensile stress- strain characterization. The experimental variables are four different quantities of silica fume, three different quantities of silica powder, three different cement types (white cement Type I, Portland cement Type V, GGBS/Portland cement Type I blend) and three different fiber volume contents (0.5%, 1.0%, and 1.5%) of straight, smooth, high strength steel fibers. Experimental results showed minor differences in mechanical behavior due to variations in the quantity of silica fume. Silica powder changes led to little difference in material behavior, suggesting that silica powder can be removed due to its high cost. UHPCs containing white cement Type I exhibited the best performance in almost all aspects of behavior including load carrying capacity, energy absorption capacity and multiple cracking behaviors, but carried the highest cost.
Specimens containing the GGBS/Portland cement Type I binder showed lower performance, but at decreased cost. UHPC specimens containing 0.5% fibers exhibited some strain hardening behavior, which became more pronounced as the fiber volume fraction increased. The results suggest that fiber volume contents of 1.0% or 1.5% could significantly reduce the chance for crack localization under dead load or working conditions, respectively, in structural applications.
3.2. EXPERIMENTAL PARAMETERS AND PROCEDURE
3.2.1. UHPC Material Properties and Cost
UHPC, depending on the types and quantity of reinforcing fibers added to the cementitious mixture, carries a high cost. Currently, commercially available proprietary blends cost
$2,000/yd3 ($2615/m3) and includes 2% steel fibers by volume (Ahlborn, 2008). This is 15 - 20 times higher than the cost of conventional concrete. Using current prices, the UHPC recently developed at the University of Michigan (Wille, 2011) carries a lower cost of materials ($516/yd3 without fibers, $1,029/yd3 with 2% fibers).
The cement used in the initial development of the UHPC in Wille et al. (2011) was a Portland Type I white cement. This cement has a high C3S content (74%), and a moderate fineness (3930 cm2/g Blaine Value) as well as a low C3A content (less than 5%). The particle sizes and costs for each UHPC constituent is listed in Figure 3-1 shows the grain size distributions for the two types of sands, F12 and F100 used in this research. The materials are obtained from reputable suppliers and the costs specified are valid for 2013 when the bulk of the research was conducted.
In Wille et al. (2011), the optimal cement to silica fume to silica powder ratio was determined to be 1 C: 0.25 SF: 0.25 SP, with a w/c ratio of 0.22 and a compressive strength of 27.8 ksi (192 MPa). Maintaining the w/c ratio established in the previous work, Table 3-2 lists the mix proportions and associated costs (without fibers) for all of the mixes considered in this work.
Cost is listed as a cost index in order to simplify the discussion later on. The cost index is simply the ratio of the mix’s cost compared to the starting mixture published in Wille (2011), based on current prices in the US. The index is a relative indicator of cost, since actual costs will vary in time and by location. The first entry, W-25-25, represents the original mix ratio in (Wille, 2011).
` Median 10% of Particles 90% of Particles
Cement 10 – 20 µm 3 µm 40 µm
Silica Fume 0.1 – 1 µm 0.1 µm 10 µm
Silica Powder 10 – 20 µm 1 µm 40 µm
F12 Sand 500 µm Larger than 300 µm Smaller than 1000 µm
F100 Sand 100 µm Larger than 50 µm Smaller than 300 µm
Silica Fume Silica Powder
SiO2 Minimum 85% SiO2 Maximum 90%
H2O Maximum 3% H2O Maximum 1%
Pozzolonic Activity Index
Minimum 105% Pozzolonic Activity Index
N/A Table 3-1: Chemical and Physical Properties of Materials
Figure 3-1 Grain Size Analysis for Sand
Cement quantity was held constant at 1306 lbs/yd3 throughout all mixes. Additionally, the admixture Advacast 575 high range water reducer was again used at a ratio of 1.35% to cement for all mixes. All mixes use the same, low w/c ratio of 0.22. Cement, silica powder, and silica
fume carried the highest costs per cubic meter. In order to lower this cost, 2 additional types of cement were identified for their reduced cost, Portland Type V and a Ground Granulated Blast Furnace Slag (GGBS) / Portland I cement blend. Table 3-3 lists the properties for the three cements used in this study. The Type I / GGBS cement blend was identified as a candidate for its exceptional long-term performance (Cheng et al., 2005).
Name White Cement
W-25-25 1.00 0.25 0.25 513 1.0
W-30-20 1.00 0.30 0.20 502 0.98
W-35-15 1.00 0.35 0.15 492
W-25-20 1.00 0.25 0.20 487 0.95
W-25-15 1.00 0.25 0.15 461 0.90
W-25-00 1.00 0.25 0.00 369 0.72
Portland Type V
PV-25-15 1.00 0.25 0.15 364 0.71
PV-25-10 1.00 0.25 0.10 338 0.66
PV-25-05 1.00 0.25 0.05 307 0.60
PV-30-05 1.00 0.30 0.05 338 0.66
PV-35-05 1.00 0.35 0.05 348 0.68
PV-25-00 1.00 0.25 0.00 282 0.55
PV-25-25 1.00 0.25 0.25 420
0.82 Portland Type I / GGBS
GG-25-00 1.00 0.25 0.00 266 0.52
GG-25-15 1.00 0.25 0.15 353 0.69
GG-25-25 1.00 0.25 0.25 405 0.79
*Matrix only, without fibers.
Table 3-2: Mixture Proportions by Weight with Cost Index
C2S + C3S %
White Cement Portland Type I 13 74 87 5 1 395
Portland Type V Cement 17 59 76 4 15 430
Type I / Slag Cement Blend 13 58 71 8 10 600
Table 3-3: Cement Properties
The cost for silica powder and silica fume was reduced through reductions in material quantities.
Ratios for SF ranged from 0.25 SF: C to 0.35 SF: C. Ratios for SP ranged from 0.00 SP: C to 0.25 SP: C. Reduction in the amount of SP was of particular interest due to its high material cost.
In some mix designs, when SP was reduced, the amounts of SF were increased since SF and SP have similar particle sizes along their particle size distribution.
3.2.2. Steel Fibers
Steel fiber reinforced concretes resist post-cracking tensile stress through the composite action between the concrete and fibers, including chemical and mechanical bonding at the interface between the two. In this study, all UHPC mixes contain 1.5% steel fibers by volume of the wet concrete. The steel fibers (Figure 3-2) used are brass coated, smooth fibers. Each fiber is 0.75 in (19 mm) long with a diameter of 0.0078 in (0.2 mm) and has a minimum tensile strength of 285 ksi (1965 MPa).
Figure 3-2: Example of the Steel Fibers Used in this Study 3.2.3. Mixing Procedure
Mixing was done using a large Hobart food-type mixer with a 2.65 gal. (10 liter) capacity (Figure 3-3). First, silica fume and the two silica sands were added into the mixer and were dry mixed for approximately 5 minutes at 136 rpm. Silica powder (if any) and cement were then added into the pan and mixed for an additional 5 minutes at 136 rpm. After this, water and the high range water reducer was gradually dispensed into the pan while the mixer was spinning.
The blend was allowed to mix for approximately 1-2 more minutes at 136 rpm. Then the mixing speed was increased to 281 rpm for approximately 5 min, or until the concrete reached an acceptable consistency. Once an adequate mixture consistency was achieved, the high strength steel fibers were added into the mixer and allowed to mix at 136 rpm until the fibers were sufficiently dispersed.
Smooth Fibers: Brass Coated 0.75” (19.2 mm) long 0.0078” (0.2 mm) dia.
Figure 3-3 Mixing process (photos courtesy of Prof. Kay Wille)
3.2.4. Tensile Strength Testing:
For the purpose of this study, a direct tension test based on AASHTO T 132-87 (2009) was chosen to test the specimens. In this test procedure, precast specimens were made and then tested
under direct tension. As shown in Figure 3-4, the specimens are supported by plates ensuring anchored and rotation-capable boundary conditions.
Figure 3-4 (a) Tensile test set up, (b) Instrumentation, (c) Specimen dimensions
Each specimen has a constant cross sectional area of 1 in2 (25 mm2) and a gauge length of 3.14 in (80 mm). The long gauge length used enables careful observation for multiple crack development. The UHPC specimens were first mixed in accordance with the procedure prescribed above. They were then poured in layers into dog-bone shaped molds to full capacity.
No vibration was used. After initial casting, the specimens were covered and stored at room temperature for 24 hours. Following this, the specimens were removed from the molds and stored in a water tank at 68° F (20° C) for 28 days. Specimens were then given time to dry
(approximately 12 hours) and then tested. For each of the mixes, at least 6 dog-bone tensile specimens were tested and the stress and strain data recorded. Figure 3-5a shows a tested specimen.
Each tensile specimen was carefully loaded into the MTS testing machine. A small preload (20%
of the matrix cracking strength) was applied to the specimen, which was then manually moved into the best-aligned position to insure uniaxial tension stress. The loading rate was set to 0.003 in/min those results in an estimated strain rate ofε!=0.0001 s-1. Following the tensile tests, the specimen crack distribution was observed and quantified. Isopropyl alcohol 99.9% was sprayed onto the specimens followed by a blue dye. The contrast in color between the dye and specimen enables a clear visualization of the crack formations.
3.2.5. Compression Testing:
The UHPC specimens were first mixed in accordance with the ratios prescribed above.
Compression specimens were poured at once into 2 in. (50 mm) cubed molds. At least 6 compression specimens were tested for each mix and their post cracking strength recorded. The cube specimens were placed into the center of the testing machine and tested in accordance to ASTM C109 (2009). Some specimens were initially precision ground in order to provide a flat surface for testing, however this was later stopped, as it did not yield noticeable differences in strengths between ground and non-ground specimens. Figure 3-5b shows a tested specimen.
Figure 3-5: Tensile and Compression Specimens Post Test
3.3. RESULTS AND DISCUSSION 3.3.1. Analysis of Data
The following naming scheme was used in order to simplify the discussion of the results. The first number corresponds to the cement type used in the mix design as discussed earlier, W for White Cement Type I, PV for the Portland V and GG for the Portland I / GGBS mix. The second letter refers to the quantity of silica fume present in the mix. The third number corresponds to the quantity of silica powder, and the fourth number corresponds to the steel fiber volume fraction of the UHPC mix design. For example, W-25-25-1.5 would indicate white cement, with 25% silica fume and 25% silica powder, containing 1.5% steel fibers by volume.
For compression, only the maximum compressive strength was considered. For the tensile testing, the test curve was broken down into the three distinct regions as discussed earlier.
Adopting the characterization scheme from Naaman (1996), the following parameters were determined: first cracking strength,
σcc, post cracking strength,σpc, strain capacity,εpc, energy
absorption capacity,g , elastic modulus, Ecc, and stress in the fibers, σ fpc. Also, the average number of cracks in the gauge length of the specimen was found. The energy absorption capacity, g, represents the energy absorption capacity prior to tension softening. This graphically corresponds to the total area under the curve up until 95% ofσpc. Experience and experimental data showed that consistent softening behavior occurred in samples beyond this point. Ecc
represents the elastic modulus of the material and is determined by the slope of the tensile curve prior to initial cracking. The value of σ fpcrepresents the average fiber tensile stress as determined using the equation proposed by Naaman (1996) and is simply the total post cracking strength divided by 90% of the fiber volume content. This 90% factor is recommended to account for the statistical variability in the experimental procedure. For each set of tensile tests, at least 3 specimen tensile plots are averaged in order to produce a single tensile response curve.
The plots are averaged at each point along the strain range. The result is then processed through a moving average filter to account for minute changes due to the sensitivity of the equipment. The average number of cracks is observed visually.
3.3.2. Overview of Results
The tensile and compressive test results produced by the experimental procedure are shown in Table 3-4. The average values between the six specimens tested per experiment were used.
Test Series Compressive
Post Cracking Strength
Energy Absorption Capacity
Fiber Tensile Stress
Average Number of
ksi (MPa) ksi (MPa) kcal/yd3 (KJ/m3) % ksi (MPa) (MPa
W-25-25-1.5 28.0 (192.7) 1.4 (9.48) 5.5 (30.2) 0.19 101.3 (698) 7.8 1.0 W-30-20-0.5 21.0 (144.7) 0.9 (6.1) 0.6 (3.3) 0.05 196.5 (1354) 1.7
W-30-20-1.0 23.7 (163.5) 1.2 (8.1) 2.7 (14.9) 0.11 131.2 (904) 5.2 0.98 W-30-20-1.5 28.3 (195.2) 1.4 (9.4) 10.0 (54.7) 0.64 100.9 (695) 8.3
W-35-15-0.5 20.9 (144.1) 0.8 (5.7) 0.5 (2.6) 0.01 182.7 (1259) 2.2
W-35-15-1.0 24.0 (165.6) 1.4 (9.7) 3.7 (20.3) 0.16 155.7 (1073) 6.2 0.96 W-35-15-1.5 28.4 (195.4) 1.3 (8.8) 4.3 (23.7) 0.07 94.9 (654) 7.8
W-25-20-0.5 25.8 (177.6) 0.7 (5.1) 0.7 (4.1) 0.08 164.4 (1133) 2.2
W-25-20-1.0 27.3 (187.8) 1.0 (7.2) 2.7 (14.9) 0.18 116.5 (803) 4.3 0.95 W-25-20-1.5 28.3 (195.3) 1.6 (10.9) 3.2 (17.5) 0.10 117.3 (808) 7.7
W-25-15-0.5 26.3 (181.0) 1.1 (7.7) 1.4 (7.6) 0.07 246.9 (1701) 2.3
W-25-15-1.0 25.8 (177.8) 1.4 (9.6) 5.6 (30.5) 0.10 154.7 (1066) 5.2 0.90 W-25-15-1.5 28.0 (192.7) 1.3 (9.2) 5.3 (29.2) 0.16 99.0 (682) 7.5
W-25-00-1.5 25.2 (173.8) 1.2 (8.2) 4.0 (21.7) 0.18 88.2 (608) 11.0 0.72 PV-25-15-0.5 20.9 (143.7) 0.9 (6.1) 1.7 (9.4) 0.06 197.7 (1362) 2.5
PV-25-15-1.0 25.0 (172.1) 1.4 (9.5) 3.2 (17.3) 0.13 152.5 (1051) 6.4 0.71 PV-25-15-1.5 26.6 (183.1) 1.6 (10.7) 6.5 (35.6) 0.11 115.4 (795) 8.3
PV-25-10-1.5 25.3 (174.4) 1.2 (8.5) 10.5 (57.2) 0.33 91.6 (631) 10.5 0.66 PV-25-05-1.5 26.4 (182.0) 1.2 (8.1) 7.6 (41.6) 0.50 86.5 (596) 10.7 0.60 PV-30-05-1.5 25.0 (172.4) 1.2 (8.2) 7.0 (38.5) 0.27 87.8 (605) 11.0 0.66 PV-35-05-1.5 25.7 (177.2) 1.0 (7.2) 3.7 (20.2) 0.24 77.5 (534) 10.5 0.68 PV-25-00-0.5 22.2 (152.9) 0.6 (4.1) 1.4 (7.4) 0.15 132.8 (915) 2.4
PV-25-00-1.0 23.5 (161.7) 1.1 (7.6) 6.4 (35.1) 0.11 122.9 (847) 5.6 0.55 PV-25-00-1.5 25.3 (174.0) 1.3 (9.0) 6.4 (35.1) 0.11 96.7 (666) 8.1
PV-25-25-1.5 27.6 (190.0) 1.3 (8.8) 3.4 (18.7) 0.15 94.5 (651) 10.0 0.82 GG-25-00-1.5 25.2 (173.8) 1.2 (8.0) 3.2 (17.6) 0.15 86.4 (595) 9.0 0.52 GG-25-15-1.5 26.2 (180.6) 1.2 (8.6) 4.4 (24.2) 0.21 91.9 (633) 10.5 0.69 GG-25-25-1.5 26.9 (185.5) 1.4 (9.4) 7.4 (40.5) 0.28 101.5 (699) 11.3 0.79
*Matrix only, no fibers.
Table 3-4: Cost and Performance Summary
29 3.3.3. Cement Type
Three different cements were tested with three different mix ratios. Figure 3-6 shows the effects of cement types on various performance parameters for mixes with 1.5% volume fiber fraction.
From Figure 3-6a, it can be seen that the compressive strength of the material varies slightly with differences in cement type. In general, the mixes containing the Portland Type V mixes perform the worst, averaging 25.9 ksi (179 MPa). Slightly better, those containing the GGBS / Portland Type I cement achieved on average 26.1 ksi (180 MPa) in compression. Those containing the White cement performed the best, averaging 27.7 ksi (191 MPa). All three cements performed above the minimum required compressive strength to qualify as UHPC, i.e. 22 ksi (150 MPa).
In tension, the average post cracking strength for each mix was also considered. From Figure 3-6b, White Cement mixes exhibited the highest tensile strength, averaging a max post cracking strength of 1.3 ksi (9.3 MPa). Portland Type V mixes averaged the lowest strengths, 1.2 ksi (8.4 MPa) and those containing GGBS / Portland Type I mixes achieved average post crack strengths of 1.3 ksi (8.9 MPa). All specimens showed at least 8 cracks in the gage length (Figure 3-6c), while specimens containing the GGBS / Portland Type I cement exhibited the most cracking. All specimens exhibited strain hardening and had a strain capacity,εpc, ranging from 0.21 to 0.24 (Figure 3-5d). Similarly, the energy absorption capacity (Figure 3-6e) and fiber tensile stress (Figure 3-6f) for all three cement types showed little variation and no clear trend between the three cement types. While specimens containing white cement performed the best in compression, all three cements showed good performance under tension and compression indicating they are all suitable for UHPC.
30 3.3.4 - Silica Powder
Figure 3-7 shows the effects of SP on various performance parameters for all mixes with 1.5%
volume fiber fraction. From Figure 3-7a, it’s seen that compressive strengths ranged from 25.1 ksi (173 MPa) at 0% SP up to 27.1 ksi (187 MPa) at 25% SP. Compressive strengths increased as SP increased up to 20%, dropping slightly as SP increased further to 25%. In tension, post cracking strengths (Figure 4b) showed little variation, with specimens containing 0% SP achieving 1.2 ksi (8 MPa) up to 1.4 ksi (9.5 MPa) for those containing 25% SP. Similarly, the average number of cracks formed showed little change from 0% SP to 25% SP. Energy absorption capacity decreased slightly from 0% SP to 20% SP, though 25% SP showed the greatest energy absorption capacity. Fiber tensile stresses essentially remained unchanged, indicating SP did not affect the ability of the fibers to transfer load. Figure 3-7 shows that significant changes in SP content resulted in minor changes in all the performance parameters.